# Impacts of Coulomb Interactions on the Magnetic Responses of Excitonic Complexes in Single Semiconductor Nanostructures

^{}

^{1}Chia-Hsien Lin,

^{1}Ying-Jhe Fu,

^{2}Ta-Chun Lin,

^{2}Hsuan Lin,

^{1}Shuen-Jen Cheng,

^{1}Sheng-Di Lin,

^{2}and Chien-Ping Lee

^{2}

^{1}Department of Electrophysics, National Chiao Tung University, Hsinchu, 30010, Taiwan

^{2}Department of Electronics Engineering, National Chiao Tung University, Hsinchu, 30010, Taiwan

^{}Corresponding author.

## Abstract

We report on the diamagnetic responses of different exciton complexes in single InAs/GaAs self-assembled quantum dots (QDs) and quantum rings (QRs). For QDs, the imbalanced magnetic responses of inter-particle Coulomb interactions play a crucial role in the diamagnetic shifts of excitons (*X*), biexcitons (*XX*), and positive trions (*X*^{−}). For negative trions (*X*^{−}) in QDs, anomalous magnetic responses are observed, which cannot be described by the conventional quadratic energy shift with the magnetic field. The anomalous behavior is attributed to the apparent change in the electron wave function extent after photon emission due to the strong Coulomb attraction by the hole in its initial state. In QRs, the diamagnetic responses of *X* and *XX* also show different behaviors. Unlike QDs, the diamagnetic shift of *XX* in QRs is considerably larger than that of *X*. The inherent structural asymmetry combined with the inter-particle Coulomb interactions makes the wave function distribution of *XX* very different from that of *X* in QRs. Our results suggest that the phase coherence of *XX* in QRs may survive from the wave function localization due to the structural asymmetry or imperfections.

**Keywords:**Quantum dots, Quantum rings, Magnetophotoluminescence, Diamagnetic shift

## Introduction

Single semiconductor nanostructures, such as quantum dots (QDs) and quantum rings (QRs), have attracted much attention due not only to their fundamental interest, but also to their potential applications in the prospective quantum information technology [1-8]. In semiconductor nanostructures, excitonic effects play a central role in their optical properties [9-15]. Electrons and holes form a variety of exciton complexes in QDs and QRs due to the enhanced Coulomb interactions by the spatial confinements. The spatial extents of excitonic wave functions thus reflect the both the combined effects of spatial confinements and the inter-particle Coulomb interactions among constituent charged carriers [9,10,13,14]. Applying a magnetic field *B* is an efficient way to probe the spatial extent of excitonic wave functions. In a magnetic field *B*, the exciton emission energy increases quadratically with *B*, i.e., the diamagnetic shift Δ*E* = *γB*^{2}, with a diamagnetic coefficient *γ* proportional to the area of the excitonic wave function. Depending on the confinement regime of the nanostructures, the measured *γ* could have different physical meanings [9]. In the strong confinement regime, where the single-particle energy dominates over the Coulomb energies, *γ* is a measure of the spatial confinement of the QDs, while the magnetic responses of inter-particle Coulomb energies only appear as correction terms to the overall diamagnetism. On the other hand, when confined excitons are in the weak confinement regime, the Coulomb energies become prominent, such that *γ* will be mainly determined by the magnetic response of the inter-particle Coulomb interactions. For exciton complexes confined in nanostructures [14,15], the diamagnetic behaviors are more complicated because of the more elaborate Coulomb interactions among the constituent charged carriers. Therefore, a systematic investigation is essential into further understanding the magnetic responses of different exciton complexes in QDs or QRs.

In this work, we report on the diamagnetic response of different exciton complexes, including neutral excitons (*X*), biexcitons (*XX*), positive and negative trions (*X*^{+} and *X*^{−}) confined in single InAs/GaAs self-assembled QDs and QRs. In QDs, the influences of imbalanced magnetic responses of Coulomb energies on the overall diamagnetisms of *X*, *XX*, and *X*^{+} are observed and discussed. As for the magnetic response of *X*^{−} in QDs, we observe an anomalous diamagnetic behavior, which cannot be described by the conventional quadratic energy shift with the applied *B*. Such anomalous behaviors for *X*^{−} can be attributed to the apparent change in the electron wave function extent after photon emission due to the strong Coulomb attraction by the hole in its initial state. In QRs, the diamagnetic responses of *X* and *XX* also show different behavior. The impacts of inherent structural asymmetry of the self-assembled QRs, as well as the inter-particle Coulomb interactions, on the distribution of *X* and *XX* wave functions are discussed. Our results suggest that the phase coherence of *XX* in QRs may survive from the wave function localization due to the structural asymmetry or imperfections.

## Experimental Details

The investigated samples were grown on GaAs (100) substrates by a molecular beam epitaxy system. For the QD sample, a layer of InAs self-assembled QDs (2.0 MLs) was grown on GaAs at 480°C without substrate rotations, yielding a gradient in area dot density ranging from 10^{8} to 10^{10} cm^{−2}. Atomic force microscopy (AFM) of uncapped samples reveals that the dots are lens shaped, with an average height and diameter of ≈2(±0.5) and ≈15 nm, respectively. The QDs were finally capped by a 100-nm undoped GaAs layer.

For the QR sample, a low-density InAs QD layer was first grown by depositing 2-ML InAs at 520°C as QR precursors. The substrate temperature was then lowered to 500°C for depositing a thin GaAs layer (1.7 nm) to cover the QD sidewalls, followed by a 50-s growth interruption for expelling the indium atoms from the QD center for the QR formation [16,17]. Surface topography of uncapped QRs has also been investigated by AFM. The area density of surface QRs is about 10^{7} cm^{−2}. Typical surface QRs have a rim diameter of 35 nm, a height of ≈1.3 nm, and a center dip of about 2 nm. The realistic dimension of the embedded QRs is expected to be much smaller [18]. We also found that the QR is anisotropic; the rim of the surface QR is higher along [].

To isolate individual QDs or QRs for optical measurements, a 100-nm-thick Al metal mask was fabricated on the sample surface with arrays of 0.3-μm apertures using electron-beam lithography. Single QD spectroscopes were carried out at 5–8 K in a specially designed micro-photoluminescence (μ-PL) setup (see Fig. Fig.1),1), where the sample was mounted in a low-temperature stage and inserted into the bore of 6-T superconducting magnet for magneto-PL measurements. A He–Ne laser beam or a cw Ti:Sapphire laser was focused onto the aperture through a microscope objective (NA = 0.5). The PL signals were collected by the same objective, analyzed by a 0.75-m grating monochromator, and detected by a liquid-nitrogen-cooled charged-coupled device (CCD) camera, which yield a resolution-limited spectral linewidth of about 60 μeV.

## Results and Discussions

### Quantum Dots

Several apertures containing only one QD have been investigated, and all of which showed similar spectral features. Typical single QD spectra consists of four dominant emission lines associated with the recombination of neutral excitons (*X*), biexcitons (*XX*), positive and negative trions (*X*^{+} and *X*^{−}). These excitonic spectra have been unambiguously identified according to power-dependent and polarization-resolved PL measurements [14]. Magneto-PL measurements have been taken on a total of seven QDs with *X* energy distributed over the range of 1,349–1,385 meV. Typical spectra selected from one particular QD are shown in Fig. Fig.2.2. When a magnetic field, *B*, was applied along the QD growth direction (Faraday geometry), each line splits into a doublet through the Zeeman effect. In addition, the average energy of each Zeeman doublet increases with the increasing *B*, known as the diamagnetic shift. In Fig. Fig.3,3, the measured diamagnetic shifts for the four excitonic emission lines are plotted as a function of *B*^{2}. For *X**X*^{+}, and *XX*, the measured diamagnetic shifts show a quadratic dependence Δ*E* = *γB*^{2}, with a clear trend of . This trend holds for all investigated dots and is a consequence of different magnetic responses of inter-particle Coulomb energies.

**a**The energy shifts of

*X*,

*X*

^{+}, and

*XX*in a QD as a function of

*B*

^{2}.

**b**The energy shifts of

*X*

^{−}as a function of

*B*

^{2}. A clear non-quadratic

*B*dependence can be seen

To explain this behavior, we consider here a 2D parabolic potential as the effective lateral confinement for both electrons and holes in the QDs, with a quantization energy of *ω*_{β} and a wave function extent of, where *β* denotes *e*or *h*and *m*_{β} are the effective masses [20,21]. The use of parabolic model simplifies the problem considerably, because of the availability of analytical formula for all Coulomb interactions being parameterized by _{β}. The inter-particle direct Coulomb energy is given by [20-22]

where . In a magnetic field *B**ω*_{β} can be replaced by the *B*-dependent hybridize frequency . In the weak-field limit, the *B*-dependent single-particle energy *Ω*_{β}(*B*) and the Coulomb energies *V*_{αβ}(*B*) can be expanded analytically as,

where is the single-particle diamagnetic coefficient, and accounts for the magnetic response of *V*_{αβ}(*B*), with a constant *k* defined as . If we take the Coulomb energies as perturbations to the single-particle energy in the strong confinement regime, the diamagnetic shift of *X* should be corrected as . On the other hand, the diamagnetic shift of *XX* will deviate from that of *X* by an amount of . Because varies as ~^{3}, a slight difference between _{e} and _{h} can lead to very different values for and . Since _{h} < _{e} and hence , we have that leads to . The same arguments can be applied to the *X*^{+} case, where is also reduced by a similar amount, in agreement with our experimental observations. The reason for can also be understood from the fact that the emission energies of *XX* and *X*^{+} are usually correlated even in different QDs [23], because their energy difference equals roughly to *V*_{ee}*V*_{eh}, which is value less sensitive to the magnetic field.

It is worth to emphasize that the systematic differences among *γ*_{X},*γ*_{XX}, andcould be observed only when _{e} and _{h} exhibit a large difference. For small InAs QDs, electron gradually lose confinement as the dot size reduces, which in turn push the electron level toward the wetting-layer continuum, resulting in a more extended electron wave function penetrating into the barrier material [24]. On the other hand, the hole wave function remains well localized in the QDs, leading to a large difference between _{e} and _{h}. For larger In(Ga) As QDs, since _{e} and _{h} are expected to be similar, the diamagnetic response of all exciton complexes will be nearly identical [13], so that the magnetic response of interparticle Coulomb energies of such strongly confined few-particle systems becomes unable to resolve experimentally.

For the case of *X*^{−} in QDs, its magnetic response shows an anomalous behavior, which does not follow the conventional *B*^{2}-dependence energy shift, as can be seen from Fig. Fig.3b.3b. Our measurements show that the *X*^{−} diamagnetic shifts in most QDs investigated are smaller and non-quadratic. To understand the peculiar behavior, the charge configurations of the initial and the final states of *X*^{−} should be considered. As depicted in Fig. Fig.4,4, the initial state of *X*^{−} consists of two electrons and one hole, which will leave one electron in its final state after recombination. The *X*^{−} diamagnetic shift thus reflects the diamagnetic responses of both the initial and final states. We have performed numerical model simulations using single-band Hamiltonian of cone-shape QDs including Hartree approximations to calculate the lateral extents of the initial-state _{e,i} and the final-state _{e,f} electron wave functions of *X*^{−}. We found that the _{e,f} is always more extended than _{e,i}. This can be realized from the presence of hole in its initial state, which contracts the electron wave function by the Coulomb attraction. As the QD sizes reduces, _{e,f} increases rapidly, due to the penetration of electron wave function into the barrier material [24]. The very extended electron becomes sensitive to the long-range Coulomb attractive potential produced by the hole in the initial state, by which _{e,i} will be contracted and become apparently smaller than _{e,f}. As a result, the final-state diamagnetic shift increases, so that the overall diamagnetic shift in *X*^{−} is reduced. This phenomenon is not expected for *X*^{+} in QDs, since the wave function extents of the initial- and final-state holes are almost identical due to the fact that hole has a larger effective mass, such that the hole wave function remains well confined even in small QDs. Therefore, the Coulomb attractive potential produced by the weakly confined electron becomes less important.

*X*

^{−}in QDs before and after photon emissions. The final-state electron is more extended due the Coulomb attraction of the hole in its initial state

Now, we explain why the *X*^{−} diamagnetic shift exhibits a non-quadratic *B* dependence. To illustrate this behavior, we consider the diamagnetic shift in the carrier’s single-particle energy and expand it in powers of *B* as,, where the quartic coefficientis negative and is given by. By taking into account the difference between _{e,i} and _{e,f}, a simple algebraic analysis for the *X*^{−} diamagnetic shift,, gives the following expression:

whereand. Because of _{h} < _{e} and,andonly have minor influences on the overall diamagnetism. Accordingly, we obtainand. Equation (3) makes clear how the difference in _{e,i} and _{e,f} can lead to anomalous diamagnetic shifts for *X*^{−}. For a normal case of _{e,i} ≈ _{e,f} = _{e}, we haveand. That is, the *X*^{−} diamagnetic shift behaves as the usual *B*^{2} dependence with a coefficient similar to that of *X*. A very interesting case occurs when, which leads to 2*γ*_{e,i} = *γ*_{e,f} and cancels out the *B*^{2} term, resulting in a dominant *B*^{4}-dependent energy shift. The energy shift shown in Fig. 3(b) exhibits both quadratic and quartic *B* dependence. Therefore, the measured curvature can also be a sensitive probe to the change in wave function extents between the initial and the final-state electrons of *X*^{−}.

### Quantum Rings

Figure Figure5a5a and and5b5b show the surface topography and line scans along [110] and [] directions of uncapped QRs. Typical single-QR magneto-PL spectra are shown in Fig. Fig.5c.5c. Two emission lines associated with the recombination from *X* and *XX* can be observed. The same measurement has been performed on a total of seven QRs with *X* emission energies ranging from 1,320 to 1,328 meV. Apart from the Zeeman splitting, both *X* and *XX* show clear diamagnetic shifts with the increasing *B*. The average diamagnetic coefficient of *X* for all the investigated QRs is. Interestingly, we found that *XX* shows a considerably larger diamagnetic coefficient with an average value of, which is more than the double of the *γ*_{X} value.

**a**Surface topography and

**b**line scans along [110] and [] directions of uncapped QRs.

**c**Typical single-QR magneto-PL spectra taken under different applied

*B*.

**d**The

*B*-dependent energy shifts of the

*X*and

*XX*.

*Solid*and

*dashed lines*are fitting curves using

**...**

The larger *γ*_{XX} indicates a more extended *XX* wave function in QRs. This is different from the case of QDs, where *γ*_{XX} is usually similar to, or somewhat smaller than, *γ*_{X} due to the different spatial extents of the electron and hole wave functions and their responses to the applied *B*. Here, we argue that the larger *γ*_{XX} is a consequence of the fact that self-assembled QRs do not have perfect azimuthal symmetry. It has been reported that buried self-assembled QRs exhibit an asymmetric craterlike shape, with a diameter substantially smaller than the ring-shaped islands on the surface of uncapped QR structures [18]. In addition, due to the preferential out diffusion of dot material along the [] direction, the embedded rim height is higher along the [110] direction, resulting in two separate potential valleys along the [110] direction, resembling a pair of connected QDs [19]. Based on the proposed shape for embedded QRs in Ref. [19], we have performed theoretical calculations for the wave function distributions of *X* and *XX* in QRs, which are shown in Fig. Fig.6.6. Although the actual shape of embedded QRs is not known exactly, the numerical model used here is still a good illustration when QRs have any structural imperfection. Using selective chemical etching to remove the GaAs capping layer may be an efficient way to reveal the structure of buried QRs [25,26].

**a**A schematic for the QR geometry with a structural anisotropy used in model calculations.

**b**and

**c**are the calculated electron wave functions of the lowest

*X*and

*XX*states. The

*dash circle*represents the rim diameter of 14 nm

The lack of rotational symmetry in the potential of embedded QRs has significant impacts on the diamagnetic responses of *X* and *XX*. For *X* confined in QRs, the height variation strongly localizes the hole in one of the potential valleys due to the large effective mass. Consequently, the electron will be bound to the same valley by the electron-hole Coulomb attraction. This means that the wave function extent of *X* is determined mainly by the confinement of the potential valley and the Coulomb interaction. Therefore, the diamagnetic response of *X* is similar to an elliptic QD.

For *XX* confined in QRs, the two holes may be separately localized in different valleys due to the strong hole–hole Coulomb repulsion. Due to the Coulomb attractions of the two separately localized holes, the electron wave functions of *XX* are more likely to spread over the two valleys and become more extended than that of *X*. Unlike *X*, the wave function extent of *XX* is determined mainly by the diameter of the embedded QRs. This explains why *γ*_{XX} is significantly larger than *γ*_{X} for QRs.

Before conclusions, we would like to comment on the implications of the larger diamagnetic shift of *XX* in QRs. Charged particles confined to a QR are expected to show the well-known Aharanov–Bohm (AB) effect due to the quantum interference of the carrier’s wave function in the ring-shaped geometry [6-8]. However, for an exciton confined in ring-like nanostructures, the AB effect is not expected to occur for such a charge-neutral composite unless the electron and hole can propagate coherently in different trajectories with a non-zero electric dipole moment [27]. This can occur naturally in type-II QD systems, where the electron and hole are spatially separated [28,29]. However, for InGaAs self-assembled QRs where both the electron and hole are confined, it is still an open question whether the excitonic AB effect can be observed. In fact, this issue is further complicated by the inherent structural asymmetry and/or imperfections presented inevitably in self-assembled QRs [18,19]. Our results suggest that the inherent structural asymmetry combined with the inter-particle Coulomb interactions tends to localize the *X* wave function and hence may smear out its phase coherence. On the other hand, due to hole–hole repulsion, the *XX* wave function is more extended and spread over the entire ring. Therefore, the phase coherence of *XX* may be more likely to survive from such wave function localizations at lower magnetic field.

## Conclusions

In conclusion, the diamagnetic response of different exciton complexes, including neutral excitons (*X*), biexcitons (*XX*), positive and negative trions (*X*^{+} and *X*^{−}) confined in single InAs/GaAs self-assembled QDs and QRs has been investigated. In QDs, we found a systematic trend ofcaused by the imbalanced magnetic responses of inter-particle Coulomb interactions, which could be observed only when the confined electron and hole wave functions exhibit a large difference in their lateral extents. Furthermore, the differencewas found to scale as the cube of its single-particle wave function extent and therefore can be a sensitive probe to the electron-hole wave function asymmetry. On the other hand, the magnetic response of *X*^{−} in QDs fell into a special regime where the conventional quadratic diamagnetic shift failed to describe its magnetic response. Our measurements show that the *X*^{−} diamagnetic shifts in most QDs investigated are even smaller and non-quadratic. Such anomalous behaviors for *X*^{−} were explained by the apparent change in the electron wave function extent after photon emission due to the strong Coulomb attraction induced by the hole in its initial state. In QRs, the diamagnetic responses of *X* and *XX* also show different behavior. Unlike single QDs, *XX* in QRs shows a considerably larger diamagnetic coefficient than the *X*. Numerical model calculations indicate that the inherent structural asymmetry and imperfection of the self-assembled QRs, combined with the inter-particle Coulomb interactions, play a crucial role in the distribution of *X* and *XX* wave functions. Our results suggest that the phase coherence of *XX* in QRs may survive from the wave function localization due to the structural asymmetry or imperfections.

## Acknowledgment

This work was supported in part by the program of MOE-ATU and the National Science Council of Taiwan under Grant Nos.: NSC-97-2112-M-009-015-MY2, NSC-97-2120-M009-004 and NSC-97-2221-E009-161. We also acknowledge the Center for Nanoscience and Technology (CNST) at National Chiao Tung University.

#### Open Access

This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.

## References

- Michler P, Kiraz A, Becher C, Schoenfeld WV, Petroff PM, Zhang L, Hu E, Imamoglu A. Science. 2000. p. 2282. COI number [1:CAS:528:DC%2BD3cXptFSnu7s%3D]; Bibcode number [2000Sci...290.2282M] [PubMed] [Cross Ref]
- Pelton M, Santori C, Vuckovic J, Zhang B, Solomon GS, Plant J, Yamamoto Y. Phys. 2002. p. 233602. Bibcode number [2002PhRvL..89w3602P] [PubMed] [Cross Ref]
- Yuan Z, Kardynal BE, Stevenson RM, Shields AJ, Lobo CJ, Cooper K, Beattie NS, Ritchie DA, Pepper M. Science. 2002. p. 102. COI number [1:CAS:528:DC%2BD38XksVeruw%3D%3D]; Bibcode number [2002Sci...295..102Y] [PubMed] [Cross Ref]
- Chang W-H, Chen W-Y, Chang H-S, Hsieh T-P, Chyi J-I, Hsu T-M. Phys. 2006. p. 117401. Bibcode number [2006PhRvL..96k7401C] [PubMed] [Cross Ref]
- Li X, Wu Y, Steel D, Gammon D, Stievater TH, Katzer DS, Park D, Piermarocchi C, Sham LJ. Science. 2003. p. 809. COI number [1:CAS:528:DC%2BD3sXmtVGqsrc%3D]; Bibcode number [2003Sci...301..809L] [PubMed] [Cross Ref]
- Lorke A, Luyken RJ, Govorov AO, Kotthaus JP, García JM, Petroff PM. Phys. 2000. p. 2223. COI number [1:CAS:528:DC%2BD3cXhsV2mtL0%3D]; Bibcode number [2000PhRvL..84.2223L] [PubMed] [Cross Ref]
- Bayer M, Korkusinski M, Hawrylak P, Gutbrod T, Michel M, Forchel A. Phys. 2003. p. 186801. COI number [1:STN:280:DC%2BD3s3mtlWjtg%3D%3D]; Bibcode number [2003PhRvL..90r6801B] [PubMed] [Cross Ref]
- Kleemans NAJM, Bominaar-Silkens IMA, Fomin VM, Gladilin VN, Granados D, Taboada AG, García JM, Offermans P, Zeitler U, Christianen PCM, Maan JC, Devreese JT, Koenraad PM. Phys. 2007. p. 146808. COI number [1:STN:280:DC%2BD2sngslGisg%3D%3D]; Bibcode number [2007PhRvL..99n6808K] [PubMed] [Cross Ref]
- Walck SN, Reinecke TL. Phys. Rev. B. 1998. p. 9088. COI number [1:CAS:528:DyaK1cXisVGitL4%3D]; Bibcode number [1998PhRvB..57.9088W] [Cross Ref]
- Bayer M, Walck SN, Reinecke TL, Forchel A. Phys. Rev. B. 1998. p. 6584. COI number [1:CAS:528:DyaK1cXhvVaru7Y%3D]; Bibcode number [1998PhRvB..57.6584B] [Cross Ref]
- Naganume Y, Arakawa Y, Tsukamoto S, Nishioka M, Sasaki S, Miura N. Phys. 1992. p. 2963. Bibcode number [1992PhRvL..69.2963N] [PubMed] [Cross Ref]
- Someya T, Akiyama H, Sakaki H. Phys. 1995. p. 3664. COI number [1:CAS:528:DyaK2MXlt12lurg%3D]; Bibcode number [1995PhRvL..74.3664S] [PubMed] [Cross Ref]
- Schulhauser C, Haft D, Warburton RJ, Karrai K, Govorov AO, Kalameitsev AV, Chaplik A, Schoenfeld W, Garcia JM, Petroff PM. Phys. Rev. B. 2002. p. 193303. Bibcode number [2002PhRvB..66s3303S] [Cross Ref]
- Tsai M-F, Lin H, Lin C-H, Lin S-D, Wang S-Y, Lo M-C, Cheng S-J, Lee M-C, Chang W-H. Phys. 2008. p. 267402. Bibcode number [2008PhRvL.101z7402T] [PubMed] [Cross Ref]
- Lin T-C, Lin C-H, Ling H-S, Fu Y-J, Chang W-H, Lin S-D, Lee C-P. Phys. Rev. B. 2009. p. 081304(R). Bibcode number [2009PhRvB..80h1304L]
- Granados D, García JM. Appl. 2003. p. 2401. COI number [1:CAS:528:DC%2BD3sXivFamu78%3D]; Bibcode number [2003ApPhL..82.2401G] [Cross Ref]
- Ling HS, Lee CP. J. 2007. p. 024314. Bibcode number [2007JAP...102b4314L] [Cross Ref]
- Offermans P, Koenraad PM, Wolter JH, Granados D, García JM, Fomin VM, Gladilin VN, Devreese JT. Appl. 2005. p. 131902. Bibcode number [2005ApPhL..87m1902O] [Cross Ref]
- Fomin VM, Gladilin VN, Klimin SN, Devreese JT, Kleemans NAJM, Koenraad PM. Phys. Rev. B. 2007. p. 235320. Bibcode number [2007PhRvB..76w5320F] [Cross Ref]
- Cheng S-J, Sheng W, Hawrylak P. Phys. Rev. B. 2003. p. 235330. Bibcode number [2003PhRvB..68w5330C] [Cross Ref]
- Cheng S-J. Phys. Rev. B. 2007. p. 075329. Bibcode number [2007PhRvB..76g5329C] [Cross Ref]
- Warburton RJ. Phys. Rev. B. 1998. p. 16221. COI number [1:CAS:528:DyaK1cXotVensb8%3D]; Bibcode number [1998PhRvB..5816221W] [Cross Ref]
- Rodt S, Schliwa A, Pötschke K, Guffarth F, Bimberg D. Phys. Rev. B. 2005. p. 155325. Bibcode number [2005PhRvB..71o5325R] [Cross Ref]
- Janssens KL, Peeters FM, Schweigert VA. Phys. Rev. B. 2001. p. 205311. Bibcode number [2001PhRvB..63t5311J] [Cross Ref]
- Wang ZM, Zhang L, Holmes K, Salamo GJ. Appl. 2005. p. 143106. Bibcode number [2005ApPhL..86n3106W] [Cross Ref]
- Ding F, Wang L, Kiravittaya S, Müller E, Rastelli A, Schmidt OG. Appl. 2007. p. 173104. Bibcode number [2007ApPhL..90q3104D] [Cross Ref]
- Govorov AO, Ulloa SE, Karrai K, Warburton RJ. Phys. Rev. B. 2002. p. 081309R. Bibcode number [2002PhRvB..66h1309G] [Cross Ref]
- Ribeiro E, Govorov AO, Carvalho W, Jr, Medeiros-Ribeiro G. Phys. 2004. p. 126402. COI number [1:STN:280:DC%2BD2c7pvVWqsA%3D%3D]; Bibcode number [2004PhRvL..92l6402R] [PubMed] [Cross Ref]
- Sellers IR, Whiteside VR, Kuskovsky IL, Govorov AO, McCombe BD. Phys. 2008. p. 136405. COI number [1:STN:280:DC%2BD1czlsVCgtg%3D%3D]; Bibcode number [2008PhRvL.100m6405S] [PubMed] [Cross Ref]

**Springer**

## Formats:

- Article |
- PubReader |
- ePub (beta) |
- PDF (399K) |
- Citation

- Diamagnetic response of exciton complexes in semiconductor quantum dots.[Phys Rev Lett. 2008]
*Tsai MF, Lin H, Lin CH, Lin SD, Wang SY, Lo MC, Cheng SJ, Lee MC, Chang WH.**Phys Rev Lett. 2008 Dec 31; 101(26):267402.* - Photoinduced dynamics in semiconductor quantum dots: insights from time-domain ab initio studies.[Acc Chem Res. 2009]
*Prezhdo OV.**Acc Chem Res. 2009 Dec 21; 42(12):2005-16.* - Temperature dependent empirical pseudopotential theory for self-assembled quantum dots.[J Phys Condens Matter. 2012]
*Wang J, Gong M, Guo GC, He L.**J Phys Condens Matter. 2012 Nov 28; 24(47):475302. Epub 2012 Oct 26.* - Ultrafast near-field spectroscopy of single semiconductor quantum dots.[Philos Trans A Math Phys Eng Sci. 2004]
*Lienau C.**Philos Trans A Math Phys Eng Sci. 2004 Apr 15; 362(1817):861-79.* - Semiconductor excitons in new light.[Nat Mater. 2006]
*Koch SW, Kira M, Khitrova G, Gibbs HM.**Nat Mater. 2006 Jul; 5(7):523-31.*

- PubMedPubMedPubMed citations for these articles

- Impacts of Coulomb Interactions on the Magnetic Responses of Excitonic Complexes...Impacts of Coulomb Interactions on the Magnetic Responses of Excitonic Complexes in Single Semiconductor NanostructuresNanoscale Research Letters. 2010; 5(4)680

Your browsing activity is empty.

Activity recording is turned off.

See more...